| ||Format||Pages||Price|| |
|4||$48.00||  ADD TO CART|
|Hardcopy (shipping and handling)||4||$48.00||  ADD TO CART|
This specification covers high-strength low-alloy structural steel plates that were produced by the thermo-mechanical controlled process (TMCP). This method consists of rolling reductions and cooling rate controls, which result in mechanical properties in the finished plate that are equivalent to those attained using conventional rolling and heat treatment processes.
This abstract is a brief summary of the referenced standard. It is informational only and not an official part of the standard; the full text of the standard itself must be referred to for its use and application. ASTM does not give any warranty express or implied or make any representation that the contents of this abstract are accurate, complete or up to date.
1.1 This specification covers steel plates produced by the thermo-mechanical controlled process (TMCP). Five grades are defined by the yield strength: 50 , 60 , 65 , 70 , and 80 . The plates are intended primarily for use in welded steel structures.
1.2 The TMCP method consists of rolling reductions and cooling rate controls that result in mechanical properties in the finished plate that are equivalent to those attained using conventional rolling and heat treatment processes, which entail reheating after rolling. A description of the TMCP method is given in .
1.3 The maximum thicknesses available in the grades covered by this specification are shown in .
1.4 Due to the special combination of mechanical and thermal treatment inducing lower rolling temperatures than for conventional hot rolling the plates can not be formed at elevated temperatures without sustaining significant losses in strength and toughness. The plates may be formed and post-weld heat-treated at temperatures not exceeding 1050°F [560°C]. Higher temperatures may be possible if proven that minimum mechanical characteristics are retained after tests with specimens in the post-weld heat treatment (PWHT) condition. For flame straightening higher temperatures can be used in accordance with the steel manufacturer’s recommendations.
1.5 If the steel is to be welded, a welding procedure suitable for the grade of steel and intended use or service is to be utilized. See Appendix X3 of Specification for information on weldability.
1.6 Supplementary requirements are available but shall apply only if specified in the purchase order.
1.7 The values stated in either inch-pound-units or SI units are to be regarded separately as standard. Within the text, the SI units are shown in brackets. The values stated in each system are not exact equivalents; therefore, each system is to be used independently of the other, without combining values in any way.
1.8 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
A6/A6M Specification for General Requirements for Rolled Structural Steel Bars, Plates, Shapes, and Sheet Piling
A673/A673M Specification for Sampling Procedure for Impact Testing of Structural Steel
ICS Number Code 77.140.50 (Flat steel products and semi-products)
UNSPSC Code 11101704(Steel)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM A1066 / A1066M-11(2015)e2, Standard Specification for High-Strength Low-Alloy Structural Steel Plate Produced by Thermo-Mechanical Controlled Process (TMCP), ASTM International, West Conshohocken, PA, 2015, www.astm.orgBack to Top